LMucko/crystallography-open-database huggingface dataset:
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 693 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003032
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 693 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5011
_cell_length_b                   8.5011
_cell_length_c                   8.5011
_cell_formula_units_Z            8
_cell_volume                     614.363
_database_code_amcsd             0003121
_diffrn_ambient_temperature      966.15
_exptl_crystal_density_diffrn    3.470
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003032
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 630 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003033
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 630 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2.001 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4947
_cell_length_b                   8.4947
_cell_length_c                   8.4947
_cell_formula_units_Z            8
_cell_volume                     612.977
_database_code_amcsd             0003122
_diffrn_ambient_temperature      903.15
_exptl_crystal_density_diffrn    3.479
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2.001 O4'
_cod_database_code               9003033
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 567 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003034
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 567 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4886
_cell_length_b                   8.4886
_cell_length_c                   8.4886
_cell_formula_units_Z            8
_cell_volume                     611.657
_database_code_amcsd             0003123
_diffrn_ambient_temperature      840.15
_exptl_crystal_density_diffrn    3.486
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003034
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 503 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003035
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 503 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4828
_cell_length_b                   8.4828
_cell_length_c                   8.4828
_cell_formula_units_Z            8
_cell_volume                     610.404
_database_code_amcsd             0003124
_diffrn_ambient_temperature      776.15
_exptl_crystal_density_diffrn    3.493
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003035
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 439 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003036
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 439 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4769
_cell_length_b                   8.4769
_cell_length_c                   8.4769
_cell_formula_units_Z            8
_cell_volume                     609.132
_database_code_amcsd             0003125
_diffrn_ambient_temperature      712.15
_exptl_crystal_density_diffrn    3.500
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003036
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 375 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003037
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 375 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4716
_cell_length_b                   8.4716
_cell_length_c                   8.4716
_cell_formula_units_Z            8
_cell_volume                     607.990
_database_code_amcsd             0003126
_diffrn_ambient_temperature      648.15
_exptl_crystal_density_diffrn    3.507
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003037
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 312 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003038
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 312 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4661
_cell_length_b                   8.4661
_cell_length_c                   8.4661
_cell_formula_units_Z            8
_cell_volume                     606.806
_database_code_amcsd             0003127
_diffrn_ambient_temperature      585.15
_exptl_crystal_density_diffrn    3.513
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003038
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 250 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003039
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 250 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4612
_cell_length_b                   8.4612
_cell_length_c                   8.4612
_cell_formula_units_Z            8
_cell_volume                     605.753
_database_code_amcsd             0003128
_diffrn_ambient_temperature      523.15
_exptl_crystal_density_diffrn    3.520
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003039
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 198 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003040
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 198 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4569
_cell_length_b                   8.4569
_cell_length_c                   8.4569
_cell_formula_units_Z            8
_cell_volume                     604.830
_database_code_amcsd             0003129
_diffrn_ambient_temperature      471.15
_exptl_crystal_density_diffrn    3.525
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003040
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 168 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003041
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 168 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4545
_cell_length_b                   8.4545
_cell_length_c                   8.4545
_cell_formula_units_Z            8
_cell_volume                     604.316
_database_code_amcsd             0003130
_diffrn_ambient_temperature      441.15
_exptl_crystal_density_diffrn    3.528
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003041
A new uranyl carbonate sheet in the crystal structure of fontanite, Ca[(UO2)3(CO3)2O2](H2O)6
Hughes, K.-A.; Burns, P. C.; American Mineralogist 88 (2003) 962–966; doi:

data_9003042
_publ_section_title
;
 A new uranyl carbonate sheet in the crystal structure of fontanite,
 Ca[(UO2)3(CO3)2O2](H2O)6
;
_journal_name_full               'American Mineralogist'
_journal_page_first              962
_journal_page_last               966
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Ca[(UO2)3(CO3)2O2]*6(H2O)
_chemical_formula_sum            'C2 H12 Ca O20 U3'
_chemical_name_mineral           Fontanite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.064
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.968
_cell_length_b                   17.276
_cell_length_c                   15.377
_cell_volume                     1851.069
_database_code_amcsd             0003131
_exptl_crystal_density_diffrn    3.984
_cod_original_formula_sum        'U3 Ca C2 O20 H12'
_cod_database_code               9003042
Bulk modulus and high-pressure crystal structures of minium, Pb3O4, determined by X-ray powder diffraction Sample: Phase III of Pb3O4 at 13.3 GPa
Dinnebier, R. E.; Carlson, S.; Hanfland, M.; Jansen, M.; American Mineralogist 88 (2003) 996–1002; doi:

data_9003043
_publ_section_title
;
 Bulk modulus and high-pressure crystal structures of minium, Pb3O4,
 determined by X-ray powder diffraction
 Sample: Phase III of Pb3O4 at 13.3 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              996
_journal_page_last               1002
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Pb3O4
_chemical_formula_sum            'O4 Pb3'
_chemical_name_mineral           Minium
_space_group_IT_number           55
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   9.3812
_cell_length_b                   6.4610
_cell_length_c                   3.3168
_cell_formula_units_Z            2
_cell_volume                     201.038
_database_code_amcsd             0003132
_exptl_crystal_density_diffrn    11.326
_cod_original_formula_sum        'Pb3 O4'
_cod_database_code               9003043
High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of anisotropic compression in pyroxenes Sample: P = 0.0001 GPa Note: altered y-coordinate of O2
Origlieri, M. J.; Downs, R. T.; Thompson, R. M.; Pommier, C. J. S.; Denton, M. B.; Harlow, G. E.; American Mineralogist 88 (2003) 1025–1032; doi:

data_9003044
_publ_section_title
;
 High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of
 anisotropic compression in pyroxenes
 Sample: P = 0.0001 GPa
 Note: altered y-coordinate of O2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1025
_journal_page_last               1032
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     NaCr(Si2O6)
_chemical_formula_sum            'Cr Na O6 Si2'
_chemical_name_mineral           Kosmochlor
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.498
_cell_angle_gamma                90
_cell_length_a                   9.5720
_cell_length_b                   8.7094
_cell_length_c                   5.2678
_cell_formula_units_Z            4
_cell_volume                     418.836
_database_code_amcsd             0003133
_diffrn_ambient_pressure         100
_exptl_crystal_density_diffrn    3.602
_cod_original_formula_sum        'Na Cr Si2 O6'
_cod_database_code               9003044
High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of anisotropic compression in pyroxenes Sample: P = 1.14 GPa
Origlieri, M. J.; Downs, R. T.; Thompson, R. M.; Pommier, C. J. S.; Denton, M. B.; Harlow, G. E.; American Mineralogist 88 (2003) 1025–1032; doi:

data_9003045
_publ_section_title
;
 High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of
 anisotropic compression in pyroxenes
 Sample: P = 1.14 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1025
_journal_page_last               1032
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     NaCr(Si2O6)
_chemical_formula_sum            'Cr Na O6 Si2'
_chemical_name_mineral           Kosmochlor
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.441
_cell_angle_gamma                90
_cell_length_a                   9.5439
_cell_length_b                   8.6831
_cell_length_c                   5.2517
_cell_volume                     415.203
_cell_formula_units_Z            4
_database_code_amcsd             0003134
_diffrn_ambient_pressure         1.14e+06
_exptl_crystal_density_diffrn    3.634
_cod_original_formula_sum        'Na Cr Si2 O6'
_cod_database_code               9003045
High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of anisotropic compression in pyroxenes Sample: P = 2.22 GPa
Origlieri, M. J.; Downs, R. T.; Thompson, R. M.; Pommier, C. J. S.; Denton, M. B.; Harlow, G. E.; American Mineralogist 88 (2003) 1025–1032; doi:

data_9003046
_publ_section_title
;
 High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of
 anisotropic compression in pyroxenes
 Sample: P = 2.22 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1025
_journal_page_last               1032
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     NaCr(Si2O6)
_chemical_formula_sum            'Cr Na O6 Si2'
_chemical_name_mineral           Kosmochlor
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.349
_cell_angle_gamma                90
_cell_length_a                   9.5173
_cell_length_b                   8.6605
_cell_length_c                   5.2374
_cell_volume                     412.051
_cell_formula_units_Z            4
_database_code_amcsd             0003135
_diffrn_ambient_pressure         2.22e+06
_exptl_crystal_density_diffrn    3.662
_cod_original_formula_sum        'Na Cr Si2 O6'
_cod_database_code               9003046
High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of anisotropic compression in pyroxenes Sample: P = 3.53 GPa
Origlieri, M. J.; Downs, R. T.; Thompson, R. M.; Pommier, C. J. S.; Denton, M. B.; Harlow, G. E.; American Mineralogist 88 (2003) 1025–1032; doi:

data_9003047
_publ_section_title
;
 High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of
 anisotropic compression in pyroxenes
 Sample: P = 3.53 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1025
_journal_page_last               1032
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     NaCr(Si2O6)
_chemical_formula_sum            'Cr Na O6 Si2'
_chemical_name_mineral           Kosmochlor
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.221
_cell_angle_gamma                90
_cell_length_a                   9.4867
_cell_length_b                   8.6323
_cell_length_c                   5.2206
_cell_volume                     408.360
_cell_formula_units_Z            4
_database_code_amcsd             0003136
_diffrn_ambient_pressure         3.53e+06
_exptl_crystal_density_diffrn    3.695
_cod_original_formula_sum        'Na Cr Si2 O6'
_cod_database_code               9003047
High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of anisotropic compression in pyroxenes Sample: P = 5.05 GPa
Origlieri, M. J.; Downs, R. T.; Thompson, R. M.; Pommier, C. J. S.; Denton, M. B.; Harlow, G. E.; American Mineralogist 88 (2003) 1025–1032; doi:

data_9003048
_publ_section_title
;
 High-pressure crystal structure of kosmochlor, NaCrSi2O6, and systematics of
 anisotropic compression in pyroxenes
 Sample: P = 5.05 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1025
_journal_page_last               1032
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     NaCr(Si2O6)
_chemical_formula_sum            'Cr Na O6 Si2'
_chemical_name_mineral           Kosmochlor
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.104
_cell_angle_gamma                90
_cell_length_a                   9.4562
_cell_length_b                   8.5997
_cell_length_c                   5.2016
_cell_volume                     404.289
_cell_formula_units_Z            4
_database_code_amcsd             0003137
_diffrn_ambient_pressure         5.05e+06
_exptl_crystal_density_diffrn    3.732
_cod_original_formula_sum        'Na Cr Si2 O6'
_cod_database_code               9003048